Output from "TOTOPOL", (version 1.92, 17 Jul 2017, Mike Treacy).

Report for the framework in file "public/tmp/tmp_194_6_110196246_hroATm.cif"

There are 144 T-atoms per unit cell
There are 288 O-atoms per unit cell

Framework density = 20.64 T-atoms per nm^3
Material density = 2.060 grams per cm^3 (excluding extra-framework material)
-------------------------------------------------------------------
-------------------------- T-O Analysis ---------------------------
-------------------------------------------------------------------
[Si] Ideal SiO distance = 1.610 Angstrom
T1  -- O1  = 1.6301 Angstrom
T1  -- O2  = 1.6283 Angstrom
T1  -- O3  = 1.6520 Angstrom
T1  -- O4  = 1.6917 Angstrom
      mean = 1.6505 Angstrom
        t1 = 0.034192  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.017935  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T2  -- O4  = 1.7454 Angstrom
T2  -- O5  = 1.6714 Angstrom
T2  -- O6  = 1.5723 Angstrom
T2  -- O7  = 1.6315 Angstrom
      mean = 1.6552 Angstrom
        t1 = 0.069358  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.045323  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T3  -- O6  = 1.5670 Angstrom
T3  -- O8  = 1.5988 Angstrom
T3  -- O9  = 1.6250 Angstrom
T3  -- O10 = 1.6776 Angstrom
      mean = 1.6171 Angstrom
        t1 = 0.048377  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.036818  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T4  -- O7  = 1.6382 Angstrom
T4  -- O11 = 1.6901 Angstrom
T4  -- O12 = 1.7490 Angstrom
T4  -- O13 = 1.6156 Angstrom
      mean = 1.6732 Angstrom
        t1 = 0.061619  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.030710  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T5  -- O10 = 1.6941 Angstrom
T5  -- O12 = 1.7610 Angstrom
T5  -- O14 = 1.6275 Angstrom
T5  -- O15 = 1.5989 Angstrom
      mean = 1.6704 Angstrom
        t1 = 0.069383  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.036756  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T6  -- O13 = 1.6069 Angstrom
T6  -- O16 = 1.6270 Angstrom
T6  -- O17 = 1.6121 Angstrom
T6  -- O18 = 1.6208 Angstrom
      mean = 1.6167 Angstrom
        t1 = 0.007227  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.007114  (0.0 is a perfect tetrahedron)

        T-O SUMMARY
          Range  = 1.5670 A <--> 1.7610 A
          Mean   = 1.6472 A
          StdDev = 0.0517 A

       t1 Range  = 0.0072 <-- 0.0484 --> 0.0694
       t2 Range  = 0.0071 <-- 0.0291 --> 0.0453

-------------------------------------------------------------------
------------------------- O-T-O Analysis --------------------------
-------------------------------------------------------------------
O1  -- T1  -- O2  = 106.787 deg; O1  -- O2  = 3 A
O1  -- T1  -- O3  = 107.652 deg; O1  -- O3  = 3 A
O1  -- T1  -- O4  = 111.755 deg; O1  -- O4  = 3 A
O2  -- T1  -- O3  = 108.953 deg; O2  -- O3  = 3 A
O2  -- T1  -- O4  = 107.820 deg; O2  -- O4  = 3 A
O3  -- T1  -- O4  = 113.633 deg; O3  -- O4  = 3 A
       106.787 deg <-- 109.433 deg --> 113.633 deg

O4  -- T2  -- O5  = 125.861 deg; O4  -- O5  = 3 A
O4  -- T2  -- O6  = 103.279 deg; O4  -- O6  = 3 A
O4  -- T2  -- O7  = 105.897 deg; O4  -- O7  = 3 A
O5  -- T2  -- O6  = 100.375 deg; O5  -- O6  = 2 A
O5  -- T2  -- O7  = 107.544 deg; O5  -- O7  = 3 A
O6  -- T2  -- O7  = 114.029 deg; O6  -- O7  = 3 A
       100.375 deg <-- 109.498 deg --> 125.861 deg

O6  -- T3  -- O8  = 109.964 deg; O6  -- O8  = 3 A
O6  -- T3  -- O9  = 105.991 deg; O6  -- O9  = 3 A
O6  -- T3  -- O10 = 119.640 deg; O6  -- O10 = 3 A
O8  -- T3  -- O9  = 119.826 deg; O8  -- O9  = 3 A
O8  -- T3  -- O10 =  96.689 deg; O8  -- O10 = 2 A
O9  -- T3  -- O10 = 105.343 deg; O9  -- O10 = 3 A
       96.689 deg <-- 109.576 deg --> 119.826 deg

O7  -- T4  -- O11 = 105.439 deg; O7  -- O11 = 3 A
O7  -- T4  -- O12 = 105.230 deg; O7  -- O12 = 3 A
O7  -- T4  -- O13 = 110.792 deg; O7  -- O13 = 3 A
O11 -- T4  -- O12 = 122.216 deg; O11 -- O12 = 3 A
O11 -- T4  -- O13 = 106.721 deg; O11 -- O13 = 3 A
O12 -- T4  -- O13 = 106.295 deg; O12 -- O13 = 3 A
       105.230 deg <-- 109.449 deg --> 122.216 deg

O10 -- T5  -- O12 = 122.868 deg; O10 -- O12 = 3 A
O10 -- T5  -- O14 = 109.963 deg; O10 -- O14 = 3 A
O10 -- T5  -- O15 = 105.905 deg; O10 -- O15 = 3 A
O12 -- T5  -- O14 = 108.957 deg; O12 -- O14 = 3 A
O12 -- T5  -- O15 = 103.854 deg; O12 -- O15 = 3 A
O14 -- T5  -- O15 = 103.337 deg; O14 -- O15 = 3 A
       103.337 deg <-- 109.148 deg --> 122.868 deg

O13 -- T6  -- O16 = 110.929 deg; O13 -- O16 = 3 A
O13 -- T6  -- O17 = 108.639 deg; O13 -- O17 = 3 A
O13 -- T6  -- O18 = 109.089 deg; O13 -- O18 = 3 A
O16 -- T6  -- O17 = 109.020 deg; O16 -- O17 = 3 A
O16 -- T6  -- O18 = 109.152 deg; O16 -- O18 = 3 A
O17 -- T6  -- O18 = 110.002 deg; O17 -- O18 = 3 A
       108.639 deg <-- 109.472 deg --> 110.929 deg

        O-T-O SUMMARY
          Range  = 96.6893 deg <--> 125.8611 deg
          Mean   = 109.4402 deg
          StdDev = 6.3033 deg

        O--O SUMMARY
          Range  = 2.4486 A <--> 3.0427 A
          Mean   = 2.6909 A
          StdDev = 0.1327 A

-------------------------------------------------------------------
------------------------- T-T-T Analysis --------------------------
-------------------------------------------------------------------
-------------------------------------------------------------------
------------------------- T-O-T Analysis --------------------------
-------------------------------------------------------------------
T1  -- O1  -- T1  = 169.660 deg ; T1  -- T1   3.2469 A

T1  -- O2  -- T1  = 128.663 deg ; T1  -- T1   2.9350 A

T1  -- O3  -- T1  = 129.831 deg ; T1  -- T1   2.9923 A

T1  -- O4  -- T2  = 171.581 deg ; T1  -- T2   3.4278 A

T2  -- O5  -- T2  = 116.767 deg ; T2  -- T2   2.8466 A

T2  -- O6  -- T3  = 105.005 deg ; T2  -- T3   2.4907 A

T2  -- O7  -- T4  = 104.862 deg ; T2  -- T4   2.5917 A

T3  -- O8  -- T3  = 171.491 deg ; T3  -- T3   3.1889 A

T3  -- O9  -- T3  = 110.951 deg ; T3  -- T3   2.6776 A

T3  -- O10 -- T5  = 160.558 deg ; T3  -- T5   3.3233 A

T4  -- O11 -- T4  = 121.589 deg ; T4  -- T4   2.9505 A

T4  -- O12 -- T5  = 145.358 deg ; T4  -- T5   3.3509 A

T4  -- O13 -- T6  = 148.121 deg ; T4  -- T6   3.0986 A

T5  -- O14 -- T5  = 142.910 deg ; T5  -- T5   3.0859 A

T5  -- O15 -- T5  = 136.950 deg ; T5  -- T5   2.9747 A

T6  -- O16 -- T6  = 123.039 deg ; T6  -- T6   2.8602 A

T6  -- O17 -- T6  = 143.299 deg ; T6  -- T6   3.0603 A

T6  -- O18 -- T6  = 124.499 deg ; T6  -- T6   2.8688 A


        T-O-T SUMMARY
          Range  = 104.8623° <--> 171.5806 deg
          Mean   = 136.3963 deg
          StdDev = 21.2676 deg

        T--T SUMMARY
          Range  = 2.4907 A <--> 3.4278 A
          Mean   = 2.9984 A
          StdDev = 0.2504 A

-------------------------------------------------------------------
------------------------ *** WARNINGS *** -------------------------
-------------------------------------------------------------------

T-T-T analysis was not conducted.

SOME T-ATOM DISTANCES ARE OUTSIDE THE NORMAL RANGE
T1  has 6 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T1  -- T1  = 2.9350 Angstrom
  T1  -- T2  = 3.4278 Angstrom
  T1  -- T3  = 3.3547 Angstrom
  T1  -- T3  = 3.3703 Angstrom
  T1  -- T1  = 2.9923 Angstrom
  T1  -- T1  = 3.2469 Angstrom
T2  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T2  -- T1  = 3.4278 Angstrom
  T2  -- T2  = 2.8466 Angstrom
  T2  -- T3  = 2.4907 Angstrom
  T2  -- T4  = 2.5917 Angstrom
  T2  -- T5  = 3.0624 Angstrom
T3  has 6 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T3  -- T1  = 3.3547 Angstrom
  T3  -- T2  = 2.4907 Angstrom
  T3  -- T3  = 3.1889 Angstrom
  T3  -- T3  = 2.6776 Angstrom
  T3  -- T1  = 3.3703 Angstrom
  T3  -- T5  = 3.3233 Angstrom
T4  -- T2  = 2.5917 Angstrom
T5  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T5  -- T2  = 3.0624 Angstrom
  T5  -- T3  = 3.3233 Angstrom
  T5  -- T4  = 3.3509 Angstrom
  T5  -- T5  = 3.0859 Angstrom
  T5  -- T5  = 2.9747 Angstrom

-------------------------------------------------------------------
---------------------- Topological Analysis -----------------------
-------------------------------------------------------------------
T1 (Si): multiplicity = 24
Coordination Sequence =
    1 4 10 22 40 63 87 111 145 194 254 313 361 408 465 542 637
TD10 = 931
Circuit symbol = 4.6_{2}.4.8_{4}.6.6_{2}
Weight = 24
Vertex symbol  = 4.6_{2}.4.8_{3}.6.6
Weight = 24

T2 (Si): multiplicity = 24
Coordination Sequence =
    1 4 12 24 37 55 80 117 162 202 243 295 356 422 491 559 631
TD10 = 937
Circuit symbol = 5.8_{2}.6.6.6_{2}.6_{2}
Weight = 24
Vertex symbol  = 5.8_{2}.6.6.6_{2}.6_{2}
Weight = 24

T3 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 23 37 58 82 109 156 208 257 312 365 418 483 563 653
TD10 = 946
Circuit symbol = 4.5.5.6_{2}.6.7_{2}
Weight = 17
Vertex symbol  = 4.5.5.6_{2}.6.8_{2}
Weight = 21

T4 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 23 39 61 89 121 157 199 248 307 371 431 498 575 656
TD10 = 953
Circuit symbol = 4.5.6.6_{2}.6.7
Weight = 16
Vertex symbol  = 4.5.6.6_{2}.6.12_{7}
Weight = 38

T5 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 24 41 63 89 122 166 217 267 312 361 426 504 585 666
TD10 = 1005
Circuit symbol = 4.6_{2}.5.6.6.7
Weight = 18
Vertex symbol  = 4.6_{2}.5.6.6.8
Weight = 22

T6 (Si): multiplicity = 24
Coordination Sequence =
    1 4 9 17 31 54 85 120 156 193 237 295 367 443 509 568 638
TD10 = 907
Circuit symbol = 4.4.4.6_{2}.6.6_{2}
Weight = 16
Vertex symbol  = 4.4.4.6_{2}.6.12
Weight = 24

<TD10> = 946.500
Average ring size = 6.1154
